evaluation of asphalt mix permeability - specific procedures for freeze/thaw and permeability...
Post on 06-Feb-2020
Embed Size (px)
EVALUATION OF ASPHALT MIX PERMEABILITY
f INAL REPORT FOR
l!I& Iowa Department '!# of Transportation
Evaluation of Asphalt Mix Permeability
Final Report for
By Roderick w. Monroe Bituminous Engineer
Iowa Department of Transportation Highway Division
Office of Materials Ames, Iowa 50010
TECHNICAL REPORT TITLE PAGE
1. REPORT NO. 2. REPORT DATE
MLR-90-2 · April 1992
3. TITLE AND SUBTITLE 4. TYPE OF REPORT & PERIOD COVERED
Evaluation of Asphalt Mix Final Report Permeability April 1992
5. AUTHOR(S) 6. PERFORMING ORGANIZATION ADDRESS
Roderick W. Monroe Iowa Department of Transportation Bituminous Engineer Materials Department
800 Lincoln Way Ames, Iowa 50010
7. ACKNOWLEDGEMENT OF COOPERATING ORGANIZATIONS
Efforts to eliminate rutting on the Interstate system have resulted in 3/4" aggregate mixes, with 75 blow Marshall, 85% crushed aggregate mix designs. On a few of these projects paved in 1988-1989, water has appeared on the surfaces. Some conclusions have been reached by visual on-sight investigations that the water is coming from surface water, rain and melting snow gaining entry into the surface asphalt mixture, then coming back out in selected areas. Cores were taken from several Interstate projects and tested for permeability to investigate the surface water theory that supposedly happens with only the 3/4" mixtures. All cores were of asphalt overlays over portland cement concrete, except for the Clarke County project which is full depth AC.
The testing consisted·of densities, permeabilities, voids by high pressure a i rmeter (HPAM), extraction, gradations, A.C. content and film thicknesses. Resilient modulus, indirect tensile and retained strengths after freeze/thaw were also done. All of the test re.sults are about as expected. Permeabilities, the main reason for testing, ranged from 0.00 to 2.67 ft. per day and averages less than 1/2 ft. per day if the following two tests are disregarded.
One test on each binder course came out to 15.24 ft/day, and a surface course at 13.78 ft/day but are not out of supposedly problem projects.
9. KEY WORDS
Rutting, Permeability, Voids
10. NO. OF PAGES
TABLE OF CONTENTS
Introduction . ..................... ; . . . . . . . . . .. . . . . . . . . . . . . . . . 1
Objective . ............... ·· . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1
Procedure . ...... .' . . . . . . .. . . . . . . . . . . . . . . . . . . . . . .. . . . . . . . . . . . . . 2
Results/ Observations. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5
Conclusions and Recommendations............................ 9
Acknowledgements. . . . . . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . . . . . . . . . 10
References ............ ·· . . . . . . .. . . . . . . . . . . .. . .. . . .. .. . . . .. .. . . . . . . . . 11
Table I - Core Permeabilities, Densities, and Voids .... 13 Table II - Summary of Resilient Modulus, Indirect ...••. 15
Tensile, and Retained Strength Averages Table III - Extracted Gradations, Asphalt cement and ••• 16
A.C. Films Table IV - Aggregate Types and Percent in Each Mixture. 17
Appendix A - Individual Core Test Results ....•••••....• 18 Appendix B - Test Formulas and Explanations ....•.•..... 27 Appendix c - Additional Project Information ........•... 34
The contents of this report reflect the views of the author and do not necessarily reflect the official views of the Iowa Department of Transportation. This report does not constitute any standard, speci- fication or regulation.
Efforts to eliminate rutting on heavy traffic asphalt pavements
have resulted in 75 blow Marshall mix designs with 3/4 inch
coarse gradations of 85% crushed materials on Interstate ace
resurfacing projects. On three of these projects paved in 1988
and 1989, water has been observed exiting through the recently
paved surface. on-site investigations consisting of coring,
trenching through the shoulder at the pavement edge, and visual
observation gave some small indication that the water may be
surface water that has penetrated the pavement through voids in
the asphalt mix and has gravitated through the pavement voids
until the right conditions of pressure, permeability, and surface
cracks exist to allow the water to exit through the pavement
The possibility of any highly permeable asphalt pavement layers
is prompting concern about future performance problems related to
asphalt stripping and/or damage due to freeze/thaw action when
these layers are saturated with water.
The objective of this study is to evaluate the permeability of
cores taken from Interstate paving projects which have exhibited
surface water as well as investigate several projects which do
not exhibit this action. Evaluation of voids, extractions,·
gradations, indirect tensile strength, resilient modulus, and
physical changes from freeze/thaw action will be conducted.
Four-inch diameter cores, through the entire thickness of asphalt
paving, were removed from the following projects.
County Project No. Milepost Station Direction Lane
Clarke IR-35-2(216)33--12-20 38.0-43.0 500 . s DR Decatur IR-35-1(54)00--12-27 0.0-7.3 125 s DR Harrison IR-29-5(58)77--12-43 75.7-90.5 1620 N DR Mills IR-29-2(32)34--12-65 38.6-43.6 745 N DR Polk IR-35-4(59)92--12-77 92.5-98.7 415 s DR Woodbury IR-29-6(87)126--12-97 128.1-141.4 1200 N DR
Ten cores were taken from each project in the outside wheel path
of the driving lane at 50 ft. intervals.
The cores were divided by sawing to separate surface and binder
layers. The following tests were performed on the specimens
taken from each project.
Specimens Tested Per Project
surf ace Binder
Density All All Permeability 3 3 Voids (HPAM) 3 3 Resilient Modulus (MR) & Indirect Tension (TI) 3 3 condition by Freeze/Thaw 3 3 TI & MR After Freeze/Thaw 3 3 Extraction & Gradation 1 1
Three additional cores were obtained from .the centerline on
Decatur and Clarke County projects to be tested for voids and
Specific procedures for freeze/thaw and permeability testing were
A falling head permeameter was built by machining parts out of
heavy, clear plastic components. A simple schematic of this
device is shown in Appendix "B". The sides of the cores had to
be sealed to stop any water from escaping and going out the sides
or edges of the cores. Colored water was used. A plastic paint
called "noryde" was used to seal the sides of the cores. The
paint did not penetrate the cores filling any voids.
Experimenting was done on cores other than the ones included in
Each core was left in the permeability machine for 120 minutes.
The water temperature and testing temperatures were done at 77°F.
The amount of water that permeated the cores was then calculated
according to the formulas found in the procedure in Appendix B.
Resilient modulus testing was conducted on six cores from each
layer of each project. Data and test parameters is included in
Appendix "A". A summary of the data is included in Table II.
Three of the cores tested for each mix were also subjected to 50
cycles of freeze and thaw and retested. The data also is
included in Table II and Appendix "A".
Indirect tensile testing was done on three cores from each layer
of each project. The formula for indirect tensile strength was
calculated as per the formula shown in Appendix B.
Some cores on which resilient modulus testing was conducted were
also used for indirect tensile. The resilient modulus is
considered a nondestructive test. This is the reason for using
some of the cores for resilient modulus, then also for indirect
tensile testing and then were further used for extraction and
The cores tested for indirect tensile were extracted and the
aggregate gradation and asphalt content was determined. The
gradations, AC content and calculated film thicknesses are shown
in Tables I and III.
The aggregate type and percent of each aggregate in each layer
for each project is shown in Table IV.
Table I shows core densities, AC contents, permeabilities and
high pressure air meter voids for specific cores for each
project and layer.
There appears to be no obvious visual correlation of air voids
and permeability. A California study and also a Georgia study
both concluded that permeability of mixes increases drastic